Density segregation of granular material in a rotating
Dale Hayter†a, Gerald Pereirab, Kurt Liffman*c, Ben Aldhamc, Sam
Johnsc, Ilija D. Sutaloc,
Geoffrey Brooks a, Paul Clearyb, Guy MetcalfecaFaculty of
Engineering and Industrial Science, Swinburne University of
VIC, AUSTRALIA 3122; bCSIRO Mathematics and Information
Sciences, Clayton, VIC, AUSTRALIA 3169;
cCSIRO Materials Science & Engineering, Highett, VIC,
Many mining operations use large quantities of water to separate
valuable minerals from less valuable gangue. This dependence on
liquid separation has an environmental impact in terms of energy
and water use and also implies a cap on production due to the
availability of water. To address these problems, the CSIRO has
developed the CSIRO Rotational Classifier, which – by using the
phenomena of rotational segregation - can quickly separate dry
granular material in terms of size and/or density without the use
of any liquids.
The purpose of this paper is to obtain a deeper understanding of
how rotational segregation can separate particles of different
densities in a rotating cylinder, free from any interstitial
fluids. This was accomplished by analyzing a cross section at the
20% fill level in a 50% full classifier, which contained a 50-50
ratio of glass and lead beads. The granular bed was sampled at
different time intervals over a 60 second period with a classifier
rotation rate of 2 rpm. These experiments resulted in a high
segregation level of 0.9 in 20 seconds and 0.95 by 60 seconds
(where a level of 1 implies full segregation). The results then
underwent image analysis and were subsequently compared to results
from a discrete element method (DEM) model where similar
segregation ratios, albeit at longer timescales, were obtained.
This study gave a further insight into the segregation process
particularly in terms of axial formation of the segregated core
which may one day be used in the separation of minerals.
Keywords: Granular Materials, Density Segregation, Discrete
Element Model, Rotational Classification
*[email protected]; phone int 613 9252 6167; fax int 613
† This study was undertaken as a partial fulfillment of the
requirements for the Degree of Bachelor of Mechanical Engineering
at the Faculty of Engineering and Industrial Science, Swinburne
University of Technology.
In many industrial applications, efficient particle separation
in terms of size and/or density is central in making the process
profitable. Separation of different materials is a common practice
in mineral mining applications. Current separation processes can
have detrimental environmental implications ranging from energy
usage with resulting greenhouse gas production through to using
increasingly scarce water resources . With environmental
concerns ever increasing, the need to come up with more
environmentally friendly ways of material separation is
Minerals of different size and density in nature are commonly
found in a dispersed state, for example, silicates in coal, heavy
minerals in minerals sands, bauxite mixed with soil. Certain grade
qualities are then required so that the end product meets a desired
specification. As such, the separation of the minerals from the
gangue is a central process in the minerals processing industry.
Common methods that industry uses to separate mineral from gangue
are, for example, vibrating screens, mechanical classifiers and
hydro-cyclone classifiers .
Biomedical Applications of Micro- and Nanoengineering IV and
Complex Systems, edited by Dan V. Nicolau, Guy Metcalfe Proc. of
SPIE Vol. 7270, 727010 · © 2008 SPIE · CCC code: 1605-7422/08/$18 ·
Proc. of SPIE Vol. 7270 727010-1
Vibrating Screens (Fig. 1a) work by having a flat porous bed
which vibrates, where the finer particles fall through the
apertures whilst retaining the larger particles. Separation of dry
materials can be attempted down to 75�m. Finer particles may cause
blinding of the sieve. One way to help sieving is to use water to
wash the screen, although fine particles may still cause problems.
A way to get around this is by using classifiers. There are 2 main
kinds of classification processes used; these are mechanical and
hydro classification .
Mechanical classifiers such as a spiral classifier (Fig. 1b)
operate with an inflow of slurry which is fed half way along the
length of the settling tank. In some spiral classifiers, the tank
has a slope of approximately 15�. The solids then settle on the
bottom of the tank which is conveyed away with a screw thread,
while the water and finer particles are washed into an overflow and
dispatched. A common problem with this method is that the spirals
impede the downward slurry movement which can result in some build
Hydro-cyclones (Fig. 1c) work by feeding the slurry in to a
conical shape cylinder. Tangential feeding of the slurry into the
device produces a vortex, which results in the heavy particles
flowing around the outside and falling down while the lighter
particles flow closer to the middle and get caught in the vortex
and flow out the top .
Fig. 1: Examples of (a) a vibrating screen (b) a spiral
classifier (c) a hydrocyclone.
A common characteristic of all these methods is the use of an
interstitial fluid to separate granular materials of different size
and density. Such a requirement may lead to difficulties in more
arid areas where the availability of water is an issue.
Alternatively, it may turn out that water is not dense enough to
separate the materials efficiently, in which case chemicals are
often used to enhance the separation process. The addition of
processing chemicals, for this and other reasons, may lead to
problems when the waste material is sent to tailings dams or when
the effluent has to be treated before it can be released to the
environment. Such storage and processing adds additional costs to
the processing system, costs that may be avoided if an interstitial
fluid is not required in the first place. One potential method for
obtaining efficient separation of dry granular materials is to use
the phenomenon of rotational segregation, which we shall discuss in
the next section.
Proc. of SPIE Vol. 7270 727010-2
Avalanching RollingICascaci ing Cataracting Centrifuging
2. ROTATIONAL SEGREGATION
Suppose that we place granular material in a cylinder, where the
central axis of the cylinder is approximately horizontal. A
characteristic criterion for the motion of solids in the cylinder
is given by the Froude number, Fr, which is the ratio of angular
acceleration to gravitational acceleration:
2�� , (1)
with � being the angular velocity, L is a characteristic length
scale, e.g., the radius of the cylinder, and g is gravitational
acceleration. This dimensionless number enables a classification of
the flow conditions of the particles, over a range of different
classifier parameters (e.g. radius and angular velocity).
Fig. 2: A schematic depiction of four different rolling regimes,
where the Froude number increases from left to right .
In Fig. 2 we show a schematic depiction of the different rolling
regimes as a function of the Froude number , where, in this
case, the relevant length scale, L, is the half length of the free
surface. In semi-quantitative terms, these rolling regimes are:
Avalanching: (0 < Fr � 10-3) when a thin layer of particles
shear, whilst the rest is in solid rotation.
Rolling/Cascading: (10-4 < Fr � 10-2) at higher speeds,
material rotates with the cylinder as a solid body until it reaches
its dynamic angle of repose � and a steady flow is obtained with a
thin cascading layer at the free surface of the rotating bed.
Cataracting: (10-2 < Fr < 1) at still higher speeds,
inertial effects cause the particles to become airborne.
Centrifuging: (Fr > 1) the particles are forced against the
wall of the rotating cylinder.
It is observed that, for the rolling regime, the granular
material often segregates in terms of size and/or density. For
material of the same density, the smaller particles go to the
centre of the granular bed, and the larger particles go to the
outside. Similarly, for particles of approximately the same size,
denser material goes to the centre of the granular bed, while less
dense material moves to the outer regions of the granular bed. In
Fig. 3, we show a schematic representation of this segregation.
This segregation has the nearly unique capability of size or
density separation without using any form of fluid.
Proc. of SPIE Vol. 7270 727010-3
Solid Body Rotation Solid Body Rotation
(b) Fig. 3 : (a) Size segregation produced by rotational motion,
where the granular material has approximately the same density.
(b) Density segregation also occurs when the material has
approximately the same size, but different densities.
The CSIRO has developed a fully automated device that uses this
segregation behaviour to separate granular material (Fig. 4). This
device, known as the CSIRO Rotational Classifier is currently
undergoing commercialization trials with the minerals equipment
manufacturer RCR Tomlinson. In this study, we wish to determine the
degree of separation that occurs within the granular bed.
Fig. 4: The CSIRO Rotational classifier.
Proc. of SPIE Vol. 7270 727010-4
Bed withsand paper
20% till level
Step Motor Shaft
3. EXPERIMENTAL AND DEM RESULTS 3.1 Equipment
The classifier used in this study is shown in Fig. 5. This
classifier was constructed out of mild steel with a inside diameter
of 110 mm and a length of 100 mm; it was designed so it would
separate at a fill level of 20%. The circular part of the
classifier was lined with an abrasive sanding paper with a grit
size of 36. This lining was used to stop the granular bed from
slipping in the classifier during rotation. The front of the
classifier was covered with Perspex. Jacking screws were used so
that the top of the classifier could be removed with as little
disruption to the bed as possible.
Fig. 5: The Classifier used in the experiments
Fig. 6: Test rig used to conduct the experiments
The classifier was mounted to a test rig shown in Fig. 6. The
test rig consisted of a variable speed motor which had a key on the
shaft to lock the classifier into place. The variable speed motor
was controlled by a control panel that could adjust the rotational
speed and the direction of rotation. The lines on the backing plate
were used to line up the classifier’s starting and finishing
positions, as well as a guide to setting the rotational speed of
Proc. of SPIE Vol. 7270 727010-5
Other equipment needed in the experiment were: a stop watch to
measure the rotation time as well as to calculate the rotational
speed of the classifier, a freezer capable of -50�C which was used
to freeze the samples, and a bottle with a plastic hose that was
used to insert water into the classifier.
For these experiments, glass and lead beads of 2 mm diameter
were placed in equal volumetric quantities into the classifier
until the classifier was 50% full. This was done to ensure no
particle dominated the segregation process and the fill ratio was
chosen so that the observed segregation would be consistent with
experimental results that are available from the literature .
Equal volumes (237 ml) of both glass and lead beads were placed
into the classifier, where the beads were randomly mixed by hand.
The degree of initial mixing was evaluated in a semi-quantitative
manner, where it was determined that there were no groups of one
particular type of particle larger than approximately 10 particles.
Other procedures could have been used to obtain a, possibly, more
constant starting point, but, due to significant time constraints,
implementing more complex mixing procedures were not practical.
The classifier was then placed on the test rig (Fig. 6), the
test rig was set to a predetermined angular rotation frequency of 2
rpm and spun clockwise for periods of 5, 10, 20, 30, 40 and 60
seconds. Rotation of the classifier always finished with the split
of the classifier and the angle of repose being parallel to one
another - to ensure the sample would cut through at the 20% level
of the classifier when it was placed on a flat, horizontal
After the experiment was completed, the sample was removed from
the test rig and placed on a horizontal surface. A plug was removed
from the Perspex window, through which the plastic hose was
inserted until it rested against the side wall of the classifier
(to minimize the affect of the water added on the beads). Water was
then added to fill the classifier to 20%; the amount of water added
was set at 53 mL. The whole classifier was then placed into a
freezer for 4 hours, freezing the beads in the classifier up to the
20% fill level. The classifier was then spilt open and the
non-frozen beads were removed to expose the core of the classified
material. The results were then photographed with a digital camera
at a set height on a tripod with two photography lamps on either
side of the sample, this ensured that the same resolution and
picture quality was achieved each time and the results were
3.3 Image Analysis
A Matlab program was written to analyse each photo. The program
took the original picture, converted it into a gray scale image,
where the gray scale image was converted into a binary (black for
lead and white for glass) image. The image was subsequently
filtered to clear parts of the photo where the pixel size was too
small, e.g., at the extremities of joining beads. Next, three masks
of a chosen image were created. The first mask was used to remove
all parts of the image that were not required for the analysis
(e.g., the. classifier drum). The second mask involved isolating
the segregated regions of black and white particles, while the
third mask traced the segregated core isolated in the second mask.
This allowed the image to be broken up in to regions of black and
white, which could be used to calculate how much area was occupied
by lead and glass beads in each segregated region. The results of
this process were then calculated to find the percentage error of
where the masks overlapped. The areas of black and white particles
in each mask were calculated and the results normalized by dividing
through by the total area of the particle region to find the ratio
Two calculations were carried out using the Matlab program, the
first of these involved using the 60 second segregated image and
transplanting it on to every other image. We then calculated the
ratio of black particles in the black region (BB), the amount of
white particle in the white region (WW) and the amount of intruder
particles in both regions (BW black in white region, WB white in
black region). This gave the segregation ratio as a function of
time which allowed an assessment of the amount of segregation that
Proc. of SPIE Vol. 7270 727010-6
To calculate the errors in the tracing during the creation of
the masks, four trials were conducted for each analysis. The
average and standard deviation were calculated. These quantities
were then used to determine the 95% confidence interval to
determine the range of values expected from the experiments. A part
of the image analysis program which generated some analysis errors
was the “im2bw” function which converted the original image to a
black and white image. Trial and error was employed in finding the
appropriate settings for identifying a particle correctly.
Unfortunately, such programs sometimes produce errors in
identifying the correct particle. To test the potential for error,
the resolution number was changed by one unit on the same image.
The error that was calculated between these images was found to be
around � 2%.
3.4 DEM Analysis
Due to the discrete, possibly irregular, nature of the granular
medium, it is not always possible to describe a granular system via
a set of continuous differential equations. As such, researchers
have developed the Discrete Element Method (DEM) as a means of
computationally describing the behaviour of granular materials. The
DEM model uses Newton’s equations of motion (rotational and
translational motion) to determine the position of the particles as
a function of time. Collisions between particles are modeled via
the agency of springs and dampers, which, in turn, provide values
for coefficients of restitution and friction between particles.
This is shown schematically in Fig. 7.
Fig. 7: Schematic depiction of particle interaction in the DEM
For this study, all collisions were deemed to be elastic, i.e.,
the coefficient of restitution was set equal to 1. The coefficient
of inter-particle friction was set at 0.5, while the coefficient of
friction between the particles and the cylinder walls was set to
1.5. The forces, velocity and position involved with each particle
were calculated by explicit numerical integration with respect to
neighbouring particles. The forces were then resolved and stored
for that instant in time. The classifier was then rotated to the
next time step (10-3 seconds), while the neighbour list was
updated. This process was continued until the classifier has been
rotated for 60 seconds. The particles and classifier dimensions
were identical to that of the experimental classifier. The DEM
model calculated the segregation ratio by removing a small area of
the classifier bed and individually counting every particle that is
in that area. This was then averaged over the whole of the
segregated region, giving the segregation ratio. The results of
this were then compared against the image analysis to validate the
4. RESULTS Although we start the experiments with equal number
of glass and lead beads, the axial and radial movement of the lead
beads during the experiment produces a final result where there are
relatively few lead beads at the front face of the classifier. This
is illustrated in Fig. 8 which shows a front view of the classifier
after 60 seconds of rotation. In Fig. 9, we
Proc. of SPIE Vol. 7270 727010-7
show the axial segregation within the classifier as a function
of time. The rotational frequency of the classifier was set to 2
rpm and the initial state of the glass and lead beads was “well
mixed”. As can be seen, segregation occurs quite rapidly with
significant segregation occurring by 20 seconds. The experimental
results are, qualitatively, very similar to the results obtained
from the DEM model, as can be seen in Fig. 10.
Fig. 8: Front view of the classifier after segregation has taken
place. The inward axial and radial movement of the lead
(black) beads relative to the glass (grey/white) beads is
Fig. 9: Axial view of segregation within the
rotational classifier using lead (black) beads and glass (white)
beads, where the classifier was rotated with a rotational frequency
of 2 rpm. The lead beads move to the centre of the bed. The
granular bed was sampled at a depth of 22mm (20% of the
Proc. of SPIE Vol. 7270 727010-8
0 10 20 40 50 GO30
Fig. 10: Discrete Element Model results for the lead
(yellow/white)/glass (blue/black) bead segregation obtained in
rotational classifier (a) axial view and (b) radial view.
Fig. 11: The segregation ratio as a function of time for the 2
rpm experimental trial. Four experimental trials were
undertaken and the error bars show the 95% confidence levels
from the experimental data. The initial segregation value was set
The segregation ratio (i.e., the proportion of lead beads in the
lead bead region) obtained from the experiments is shown in Fig.
11, where it should be noted that the initial value at zero time
was, accidentally, not measured, but was set to 0.5. As can be
seen, the classifier becomes nearly fully segregated within twenty
seconds, which, at 2 rpm, is two thirds of the rotational period of
the classifier. The segregation ratio as obtained from the DEM
model for three rotational frequencies (1, 2 and 4 rpm) is shown in
Fig. 12. The DEM results suggest that the system becomes fully
segregated after sixty seconds or two revolutions of the
classifier. This discrepancy will be subject to further study.
Proc. of SPIE Vol. 7270 727010-9
0.420 40 60
Angular velocityin revs/mm.
Fig. 12: Segregation Ratio as a function of time as modeled by
DEM for three rotational frequencies (�): 1, 2 and 4 rpm.
5. CONCLUSION This study analyzed the segregation of particles
of different densities in a rotational classifier. This was done to
determine the feasibility of using a dry rotational classifier in
the separation of minerals in the mining industries. Dry separation
technologies have a major advantage over current separation
techniques which either use a large quantity of water or use
chemicals, both of which can have an impact on the environment.
We examined the segregation obtained at the 20% fill level of a
classifier in the axial direction. The results of this experiment
show that at a rotational frequency of 2 rpm a high segregation
percentage of 90 to 95% occurs in a core region after about 20
seconds. The speed and quality of this segregation would suggest
that rotational classification may have some commercial potential
in the mining and other relevant industries, with the caveat that
differently sized particles and moisture content have not been
considered. The effects of such parameters on the segregation would
need to be evaluated before the technology could be used in a
Comparing the experimental results to those obtained from the
DEM model indicated qualitative agreement between the two data
sets. However, the experimental results appear to indicate faster
separation relative to the DEM results. The source of this
discrepancy needs to be determined before we can be fully confident
that the DEM model is replicating reality in a reasonably accurate
 Norgate, T. E., Jahanshahi, S. and Rankin, W. J., “Assessing
the environmental impact of metal production processes,” Journal of
Cleaner Production, 15, 838-848, (2007).
 Gupta, A., and Yan, D. S., [Mineral Processing Design and
Operations an Introduction], Elsevier (2006).
 Ottino, J. M., and Khakhar, D. V., “Mixing and segregation
of granular materials,” Annual Review of Fluid Mechanics, 32,
 Jain, N., Ottino, J. M., and Lueptow R. M., “Regimes of
segregation and mixing in combined size and density granular
systems: anexperimental study,” Granular Matter, 7, 69-81,
Proc. of SPIE Vol. 7270 727010-10